Download presentation

Presentation is loading. Please wait.

Published byMadelynn Hurlbutt Modified about 1 year ago

1
Assessment of Plastic Flow and Fracture Properties with Small Specimen Test Techniques for IFMIF-Designed Specimens P. Spätig 1, E. N. Campitelli 2, R. Bonadé 1, N. Baluc 1 1) Fusion Technology-CRPP-EPFL, Association EURATOM-Confédération Suisse 2) Laboratory for Materials Behavior, Nuclear Energy and Safety Research Department, Paul Scherrer Institute, Switzerland 20 th IAEA Fusion Energy Conference Vilamoura, Portugal November 1-6, 2004

2
Specificity of neutron fusion irradiation (1) neutron < 1 MeV:(n, n) elastic and inelastic scattering (n, ) capture Primary knock-on atom energy up to about 40 keV. ********************************************************* neutron > 1 MeV:Transmutation reactions come into play (n, p), (n, d) (n, t) (n, He)… H, and He production Primary knock-on atom energy up to several hundreds keV. For the fusion neutron spectrum, different nuclear reactions with the nuclei of the surrounding materials are possible:

3
Specificity of neutron fusion irradiation (2) Expected dose at the end of life of a reactor. Fusion reactor first wall: 100 to 200 dpa (displacement per atom) with a helium production of about 10 appm He/dpa and 40 appm H/dpa. Fission reactor vessel: 0.1 dpa without He.

4
The International Fusion Materials Irradiation Facility (IFMIF) An irradiation facility that reproduces as close as possible the fusion neutron environment is necessary to qualify and develop structural, functional, breeding, magnet… materials.

5
IFMIF requirements … … to be fulfilled in terms of the neutron spectrum are mediated by: 1.He and H production rates as well as other transmutation reaction rates. 2.The damage production function W(T), which characterized the primary recoil energy spectrum, has to mimic that of a fusion reactor.

6
Comparison of the neutron spectrum and the damage production function -W(T) - between IFMIF and DEMO in its current design W(T) function in the blanket represents the fraction of damage energy released by all PKA recoils with recoil energies lower than T (MeV). A. Möslang et al. Comprehensive Design Report (2004) Different neutron spectra

7
IFMIF - Schematic layout A. Möslang et al Nucl. Fusion IFMIF is an accelerator based D-Li neutron source

8
IFMIF Details of the target area and test cell The high-flux test module volume is about 0.5 L.

9
Small specimen test techniques (SSTT) u Many small specimen techniques have been developed by the fusion material research community. Needs are mainly dictated by: » Small volume irradiation facilities like IFMIF (but also accelerators, fission reactors) u A large variety of specimen geometries have been developed. This includes either a scaling down of standard test specimens or the development of new tests for small specimens (punch tests with TEM discs).

10
Small specimen test techniques (SSTT) u Development of these specimens and techniques has led to collateral advantages: » Minimize temperature uncertainties and flux gradient effects » Optimize us of limited amounts of materials » Reduce dose during PIE u Application of SSTT forces the community to solve the issues related to transfer of the test data to structural integrity assessment.

11
Example of SSTT specimens for IFMIF

12
Irradiation effect on the tensile properties of tempered martensitic steels Yield stress increase y (T irr, ,d /dt…) Uniform elongation reduction u (T irr, ,d /dt…) resulting from the build- up of irradiation induced defects in the matrix (I- loops, micro-voids and precipitates). F82H steel, T test = T irr = 293K

13
Irradiation effect on the fracture properties of tempered martensitic steels Tempered martensitic steels (bcc) exhibit a ductile-brittle transition Two major effects of irradiation: 1) Shift of the brittle regime to higher T + T o 2) Decrease of fracture toughness in the ductile regime K.

14
Simplified roadmap to model fracture toughness in the transition (brittle) region Fracture testing Tensile testing Critical applied stress intensity factor K IC, versus temperature FEA, - fields at crack tip Critical condition for cleavage, ( *-A*) for K IC Constitutive behavior ( , d /dt, T) Modeling of K(T) curve in the transition

15
Thus we need to: ( ) 1.Establish the true stress - true strain relationship ( ) over a significant plastic deformation range. 2.Understand the plastic flow with physically-based models in order to… 3.…gain insight into the micromechanisms controlling fracture. Therefore the fracture properties are intrinsically related to the plastic flow described by a constitutive law ( ) usually determined by plain tensile test.

16
How to establish ( ) for irradiated materials? Owing to the low uniform elongation measured with tensile tests after irradiation, this type of test is usually not suitable to determine ( ) for irradiated material. F82H steel, T test = T irr = 293K

17
Non-standard small ball punch test R1 = 1 mm R2 = 0.2 mm D1 = 1 mm, D2 = 1.5 mm D3 = 3 mm T = mm A 3 mm diameter disk is clamped between two dies and is deformed by bending. The load-deflection L- curve is recorded. Eurofer97 tested at room temperature

18
Finite element axisymmetric model Model implemented in ABAQUS The ball and dies are rigid bodies. The disk was modeled with 2000 axisymmetric linear reduced integration elements (CAX4R). A force is applied between the upper and the lower dies during the deformation, this prevents the specimen from slipping. Friction between these dies and the disk constrains the latter in the same way as in the actual experimental device. The calculations were run by imposing the vertical displacement of the ball.

19
On the determination of the ( ) relationship from small ball punch test 1. Experimental load - deflection curve L(N) - D(mm) ( ) relationship to be determined. Make a reasonable guess and use it as input for FE simulation 3. FE simulation of the punch test 4. Calculated load - deflection curve L(N) - (mm) 5. Comparison, Does the calculated curve match the experimental one? YES, acceptable NO, modify ( ) and reiterate

20
Validation of the FE model for the tempered martensitic F82H-mod steel Exp. data range Equivalent plastic strain in the disk reaches about 0.6, so the ( ) relationship measured with tensile test had to be extrapolated. Tensile test curveSmall ball punch test curve The non-saturating ( ) curve fits better the punch curve. Extrapolation range PyPy 0.2 Search a calibration between the yield load P y and the yield stress 0.2

21
Calibration between the yield stress 0.2 (tensile test) and yield load P y /t 2 (punch test) 0.2 MPa = 375 P y /t 2 (kN/mm 2 ) 0.2 :yield stress (MPa) P y :yield load (kN) t:specimen thickness (mm) A universal empirical linear relationship between 0.2 and P y /t 2 was found for a variety of bcc materials with different morphologies covering a wide range of stresses.

22
What irradiation induced changes in the ( ) constitutive behavior can we expect to measure from punch tests? A irradiation-hardening of 300 MPa was selected, followed by three different post-yield behaviors. The corresponding punch curves were calculated. averaged flow stress spt slope Clearly, there is a one-to-one correspondence between ( ) and F - A calibration between the averaged flow stress and punch curve slope is proposed.

23
Investigation of the plastic flow properties from small ball punch test Also in this case, an empirical linear relationship between the SPT curve slope and the averaged flow stress was found. The strain-capacity can therefore be estimated form the punch test.

24
Specimen size effect on fracture toughness Compact tension Bend bar 1.The smaller the specimens, the higher the measured fracture toughness. 2.Large scatter in the transition, statistical nature of cleavage.

25
Fracture Much of the recent work addresses use of Master Curve-Shift (MC- T) method for fracture toughness. K(T) has a constant shape and is indexed at an absolute temperature T o for K = 100 MPa m 1/2. KeKe T K MC (T) KRKR K small specimens (T) TgTg T i rr K irr (T) K e (T) = K MC (T-[T o + T]) T = T i + T g + T sr + T m ToTo

26
Reconstruction of K(T) curve, local approach based on a critical criterion *-A* to trigger cleavage. Cleavage criterion a critical stress * encompassing a critical area A* u Small specimens are used to develop micromechanics-based approach to fracture: » Constitutive equations for use in Finite Element calculations of crack tip stress/strain fields » Local fracture parameters -- e.g., critical stress ( *) critical area (A*) descriptions of cleavage fracture These can in turn be used in combination with Finite Element Modeling (FEM) to estimate T g for various specimen/component sizes and geometries. A* **

27
Drastic effect of the details of ( ) on the critical K to reach the criterion *-A* Constitutive relationship * = 2000 MPa - A*= 1x10 -8 m 2 ( p ) unirradiated 100 MPa m 1/2 ( p ) irradiated Nr MPa m 1/2 ( p ) irradiated Nr MPa m 1/2 ( p ) irradiated Nr MPa m 1/2 A* **

28
Summary The available irradiation volume of IFMIF makes the development and use small specimen test techniques (SSTT) necessary. It was shown that SSTT like: 1.the non-standard ball punch test, 1.fracture testing with sub-sized specimens that do not meet the ASTM requirements are pertinent to investigate the fundamental plastic flow and fracture properties and are applicable to the design of defect tolerant fusion structures if and only if an appropriate approach based on physically-based models is used to rationalize the experimental results.

29
The success in the search for fusion materials depends on the existence of a suitable neutron source - IFMIF - and on our ability to develop predictive models of the irradiation environment on the material properties. Conclusion

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google